DE. A. MATTHIESSEN ON THE SPECIFIC GEAVITY OF ALLOTS. 
181 
Table II. (continued.) 
Tin-Cadmium Series (determined by A. Matthiessen). 
i 
! AUoy. 
Mean 
Specific gravity 
found. 
of 
T. 
Calculated specific 
gravity, from 
volume. 
Ratio of volumes, 
V+Vi 
V 
SngCd 
7*434 
12*7 
7-456 
1-0029 
Sn^Cd 
7*489 
15-0 
7*524 
1*0047 
SnjCd 
7*690 
12-9 
7*687 
0-9996 
Sn Cd 
7*904 
13*2 
7*905 
0-9999 i 
Sn Cdj 
8-139 
11-1 
8*137 
0-9998 
Sn Cd^ 
8-336 
14-5 
8-335 
0-9999 I 
Sn Cdg 
8-432 
15-0 
8-424 
0*9990 1 
Tin-Bismuth Series (determined by Mr. M. Carty). 
Sn^ Bi 
7*438 
19*9 
7-438 
1-0000 
Sng Bi 
7*943 
20*0 
7*925 
0-9977 
Sug Bi 
8*112 
14-2 
8-071 
0-9949 
Sn^ Bi 
8*339 
13-9 
8*305 
0-9959 
Sng Bi 
8-772 
12-6 
8-738 
0-9961 
Sn Bi 
9*178 
15*9 
9*132 
0-9950 
Sn Big 
9*435 
15-0 
9*423 
0-9987 
Sn Bi^ 
9*614 
12*7 
9*606 
0-9991 
Sn Big 
9*673 
15*2 
9-674 
0-9999 
Sn BijQ 
9*737 
19*8 
9*731 
0*9994 
Sn Bi,g 
9*774 
23*0 
9*792 
1-0019 
Sn Bijj 
9*803 
22-8 
9-801 
0-9998 
Sn Bigg 
9*811 
19*0 
9*807 
0-9996 
Sn Bigg 
9-814 
19*5 
9*812 
0-9998 
Biggg 
9*815 
18-1 
9*818 
1-0003 
Tin-Silver Series (determined by Dr. M. Holzhanist). 
§"36^?+ 
7*421 
18-6 
7*404 
0-9977 
SnjoAg 
7*551 
18*8 
7*307 
0-9941 
Sn„Ag+ 
7-666 
18*4 
7*603 
0-9918 
Sng Ag+ 
7*963 
19*3 
7*858 
0*9868 
Sn4 Ag+ 
8-223 
16-3 
8*071 
0-9815 
Sn.^ Ag 
8-828 
13-8 
8-543 
0-9677 
Sn Ag 
9*507 
12-9 
9 086 
0-9558 
Sn Agg 
9*953 
14-8 
9*585 
0-9630 
Tin-Lead Series (determined by Mr. C. Long). 
Sug Pb 
7*927 
15-2 
7*948 
1*0027 
Sn^ Pb 
8-188 
16-0 
8*203 
1-0018 
Sng Pb 
8-779 
17*2 
8-781 
1-0002 
Sn Pb 
9-460 
15-5 
9*474 
1-0015 
Sn Pbg 
10-080 
14-8 
iO-136 
1-0055 
Sn Pb^ 
10-590 
14-3 
10-645 
1-0052 
Sn Pbg 
10-815 
15-6 
10-857 
1-0039 
Tin-Mercui-y Series (determined by Dr. M. Holzmann). 
Sn2Hg 
9-362 
9*9 
9*282 
0-9914 
Sn Hg 
10-369 
14-2 
10-313 
0-9946 
Sn Hgg 
11-456 
11-3 
11-373 
0-9927 
